The critical current of superconductors: an historical review


 Esther Harmon
 1 years ago
 Views:
Transcription
1 LOW TEMPERATURE PHYSICS VOLUME 27, NUMBER 9 10 SEPTEMBER OCTOBER 2001 The critical current of superconductors: an historical review D. DewHughes* Oxford University, Department of Engineering Science, Parks Road, Oxford OX1 3PJ, UK Submitted May 4, 2001 Fiz. Nizk. Temp. 27, September October 2001 The most important practical characteristic of a superconductor is its critical current density. This article traces the history of the experimental discoveries and of the development of the theoretical ideas that have lead to the understanding of those factors that control critical current densities. These include Silsbee s hypothesis, the Meissner effect, the London, Ginsburg Landau, and Abrikosov theories, flux pinning and the critical state, and the control of texture in hightemperature superconductors American Institute of Physics. DOI: / INTRODUCTION The most important characteristic of any superconductor, from the viewpoint of practical applications, is the maximum electrical transport current density that the superconductor is able to maintain without resistance. This statement is equally true for largescale applications, such as power transmission lines, electromagnets, transformers, faultcurrent limiters and rotating machines, as well as for smallscale electronic applications such as passive microwave devices and devices based on the Josephson effect. High lossless current densities mean that machines and devices can be made much smaller and more efficient than if made with a conventional resistive conductor. This was realized immediately upon the discovery of superconductivity; Onnes himself speculating on the possibility of magnet coils capable of generating fields of 10 5 G. 1 These early hopes were dashed by the inability of the thenknown superconductors to sustain substantial currents, and applied superconductivity did not become a commercial reality until alloy and compound superconductors based on the element niobium were developed around In the two following decades, intensive effort, primarily by metallurgists, led to the understanding of the factors that control critical currents and to the development of techniques for the fabrication of complex multifilamentary flexible conductors at economic prices. The discovery of the mixed copper oxide hightemperature superconductors initially produced a disappointment similar to that experienced by the pioneers of superconductivity. The superconducting characteristics of these materials introduced a new set of obstacles to achieving current densities of magnitudes sufficient for practical device applications. The difficulties involved in producing long lengths of highcurrent conductor from these materials are only just being overcome. This article is not intended to be a review of everything that is known about critical currents in superconductors. Its aim is to trace the historical development of the understanding of the factors that control critical current density in superconductors. The significant experimental facts and theoretical ideas that have contributed to the present level of knowledge will be outlined, and the crucial contribution to the topic made by Lev Vasilievich Shubnikov will be highlighted. THE EARLY YEARS Within two years of his discovery of superconductivity in mercury, Onnes recorded that there was a threshold value of the current density in mercury, above which the resistanceless state disappeared. 3 This critical value was temperature dependent, increasing as the temperature was reduced below the critical temperature, according to the expression 4 J c T J c 0 T c T /T c. A similar behavior was observed in small coils fabricated from wires of tin and lead. 5 These represent the firstever superconducting solenoids. Also noticed was the fact that the critical current density in the coils was less than that observed in short, straight samples of wire. This is the first instance of the phenomenon that was to plague the designers of superconducting magnets. The following year Onnes reported on the influence of a magnetic field on the superconducting transition in lead: The introduction of the magnetic field has the same effect as heating the conductor. 6 The existence of a critical magnetic field, above which superconductivity ceased to exist, was demonstrated. Surprisingly, perhaps because of the intervention of the First World War, Onnes failed entirely to make the connection between the critical current and the critical magnetic field. This connection was left to be made by Silsbee, as a consequence of his examining all of Onnes published reports in great detail. Silsbee s hypothesis states, The threshold value of the current is that at which the magnetic field due to the current itself is equal to the critical magnetic field. 7 From outside a conductor of circular crosssection, carrying a current I, the current appears to flow in a dimensionless line down the middle of the conductor. At a distance r away from a line current, there is a tangential magnetic field of strength H r I/2 r. If the radius of the conductor is a, then the field at the surface of the conductor will be H a I/2 a X/2001/27(9 10)/10/$ American Institute of Physics
2 714 Low Temp. Phys. 27 (99 10), September October 2001 D. DewHughes and the critical current, according to Silsbee s hypothesis, will be I c 2 ah c. It should be noted that the critical current is thus not an intrinsic property of a superconductor, but is dependent upon the size of the conductor, increasing as the diameter of the conductor is increased. Conversely, the critical current density, also size dependent, decreases as the diameter of the conductor is increased: J c 2H c /a. The experimental confirmation of Silsbee s hypothesis had to wait until after the end of the war. Both Silsbee 8 and the Leiden laboratory 9 carried out experiments on wires of differing diameters that did indeed confirm the correctness of the hypothesis. Tuyn and Onnes stated, On the faith of these results obtained up till now we think we may accept the hypothesis of Silsbee as being correct. Silsbee s summary was, It may therefore be concluded that the results of these experiments can be completely accounted for by the assumption of a critical magnetic field, without making use of the concept of critical currents. Equation 2 is valid whatever the actual distribution of the current inside the conductor, and therefore Eq. 4 also holds for a hollow conductor of the same external radius. An ingenious extension of the Leiden experiments was to measure the critical current of a hollow conductor in the form of a film of tin deposited on a glass tube. An independent current was passed along a metal wire threaded through the tube. Depending on the direction of this current the critical current of the tin was either augmented or decreased, as the field at its surface resulted from both currents in the tin film and in the wire. This reinforced the validity of Silsbee s hypothesis. At the same time, the Leiden laboratory was also making a study of the temperature dependence of the critical field in tin, with the result: 9,10 H c T H c 0 1 T 2 T c Also hysteresis in the superconducting transition was observed for the first time. 11 Hysteresis was subsequently observed in indium, lead, and thallium, and it was suggested that it might be an effect of purity, strain, or crystalline inhomogeneity. 12 It was decided that measurements on single crystals would be desirable, and in 1926 Shubnikov, who at that time was an expert in the growth of single crystals, joined the Leiden laboratory on a fouryear secondment. Meanwhile, in 1925, a new liquid helium laboratory was established at the Physikalische Technische Reichsanstalt in Charlottenberg. Chosen as the head of this laboratory was a former student of Planck, Walther Meissner. Meissner immediately instituted a program of work on superconductivity, but in order to avoid conflict with the Leiden group, this program concentrated on the superconducting transition metals, in particular tantalum and niobium. At Leiden attention had now turned to binary alloys, one constituent of which was a superconductor and the other a nonsuperconductor. Not only did alloying often raise the transition temperature to well above that of the superconducting element, but these alloys also exhibited very high critical fields. These investigations culminated in the discovery that the Pb Bi eutectic had a critical field of about 20 kg at 4.2 K, and its use to generate high magnetic fields was proposed. 13 This was actually attempted at the Clarendon laboratory in Oxford, to which Lindemann had recruited Simon, Kurti, and Mendelssohn as refugees from Nazi Germany. The attempt failed, as did a similar one by Keesom in the Netherlands. Resistance was restored at levels of magnetic field more appropriate to pure elemental superconductors. The conclusion was that the Silsbee s hypothesis was not valid for alloys. 14 The studies on tin single crystals at Leiden had produced the puzzling results that, in a transverse field, resistance was restored at a value of field onehalf of the critical field when the field was applied parallel to the axis of the crystal. 15 Von Laue, better known for his xray work, realized the significance of this result and suggested that it would be profitable to explore the distribution of magnetic field in the neighborhood of a superconductor. 16 Meissner had already interested himself in this problem; he and others had considered the possibility of a supercurrent being essentially a surface current. In 1933 Meissner and Ochsenfeld published the results of their experiments in which they measured the magnetic field between two parallel superconducting cylinders. The enhancement of the field as the temperature was lowered below the critical temperature of the cylinders indicated that flux was being expelled from the body of the superconductors. 17 Shubnikov had left Leiden in 1930 to take up a position at the Ukrainian Physicotechnical Institute in Kharkov, where he shortly became the scientific director of the newly established cryogenic laboratory. Liquid helium became available in the laboratory in 1933, and in the following year Rjabinin and Shubnikov gave confirmation of the Meissner effect in a rod of polycrystalline lead. 18 The importance of this discovery of the Meissner effect to the understanding of superconductivity cannot be overemphasised. A perfect conductor will exclude flux if placed in an increasing magnetic field, but should retain flux if cooled to below its transition temperature in a magnetic field. The Meissner effect is the expulsion of flux from the body of a superconductor when in the superconducting state. The transition from the normal state to the superconducting state is path independent, and the superconducting state is thermodynamically stable. Armed with this knowledge it was possible to develop phenomenological theories of superconductivity. Being the more stable state below the transition temperature, the superconducting state has a lower energy than the normal state. It is possible to show, from simple thermodynamics, that the energy per unit volume of the superconducting state relative to the normal state is G ns 1 2 0H c 2. This is in fact just the energy required to exclude the magnetic field from the superconductor. Two phenomenological theories followed almost immediately from the discovery of the Meissner effect. The two 7
3 Low Temp. Phys. 27 (99 10), September October 2001 D. DewHughes 715 fluids model of Gorter and Casimir 19 was able to describe the influence of temperature on the properties of the superconducting state, and it is similar to the theory for liquid helium below its lambda point. In particular, the temperature dependence of the critical magnetic field, Eq. 6, can be derived from the twofluid model. The London theory deals with the effect of magnetic fields upon the superconducting properties, and describes the spatial distribution of fields and currents within a superconductor. 20 The Londons showed that flux was not totally excluded from the body of a superconductor, but that it penetrated exponentially, from the surface, decaying over a characteristic length, the penetration depth H r H 0 exp r/. Associated with the gradient in field is a current J r H r 8 H 0 exp r/. 9 Note that this current has a maximum value at the surface, r 0, equal to H c (0)/. This is the maximum current density that a superconductor can tolerate, and for lead, for example, with a critical field at 4.2 K of A/m and a penetration depth of 35 nm, this maximum current density is A/m 2. Another important result of the London theory was the conclusion that magnetic flux trapped by holes in a multiply connected superconductor, or within the body of the superconductor, must be quantized. The quantum of magnetic flux was shown to be 0 h/q, where h is Planck s constant and q is the charge of the carrier associated with superconductivity. The groups at Oxford, Leiden, and Kharkov continued their studies on alloys. The addition of 4% Bi to Pb was sufficient to completely trap magnetic flux when an external field was reduced from above the critical field to zero. 21 In alloys of Pb Ti and Bi Ti, in increasing applied fields, flux began to penetrate at fields well below those at which resistance was restored. 22 Rjabinin and Shubnikov s work on single crystals of PbTl 2 clearly demonstrated the existence of two critical fields. Below the lower critical field, H k1 in their notation, the alloy behaved as a pure metal superconductor, with no flux penetration. Above H k1 flux began to penetrate; penetration was completed at the upper critical field H k2, at which point the resistance was restored. On reducing the field some hysteresis was observed, with a small amount of flux remaining in the sample at zero field. 23 Thus was typeii superconductivity recognized. It also appeared that Silsbee s hypothesis was obeyed by alloys, if the critical current was related to the lower critical field. Mendelssohn essayed an ingenious explanation for the two critical fields, the hysteresis and flux trapping, with his sponge model. 24 This model postulated that a sponge or threedimensional network of superconductor with a high critical field permeated the main body of the superconductor with a lower critical field. Flux penetration would commence once the external field exceeded the critical value for the body of the superconductor, but penetration would not be complete until the critical field of the sponge was reached. On reducing the field, the meshes of the sponge would trap flux, accounting for hysteresis. The nature of the sponge was not specified, but it was assumed that the meshes were of a dimension small compared to the penetration depth. Gorter 25 produced an alternative proposal, that the alloy superconductors subdivided into extremely thin regions, rather like a stack of razor blades, parallel to the applied field. This suggestion is remarkable in the light of Goodman s lamellar theory for typeii superconductivity. 26 However, even more prescient was Gorter s notion of a minimum size for the superconducting regions, foretelling the later concept of the coherence length. Because in an ideal superconductor the flux expulsion is not complete, some surface penetration occurring, the energy required to expel the flux is less than that given by Eq. 7, and the actual critical field is slightly higher than that predicted from complete expulsion. This effect is barely noticeable in bulk superconductors, but can become appreciable when at least one dimension of the superconductor is comparable to, or smaller than, the penetration depth. H. London 27 showed that the critical field for a slab of superconductor, of thickness d, in an external field parallel to the faces of the slab is given by H f H c 1 d tanh d 1/2. 10 When d is small compared to, this reduces to H f ) d H c. 11 Thus thin films can remain superconducting to higher fields, and carry higher currents, than can bulk superconductors. This suggestion was verified experimentally by Shalnikov in London suggested that, if the surface energy between normal and superconducting regions was negative, the superconductor would split into alternate lamellae of normal and superconducting regions, as suggested by Gorter. Fine filaments, of diameter less than the coherence length, are expected, by similar arguments, to have a higher critical field than that of the bulk. The Mendelssohn sponge could well be a mesh of fine filaments, with superconducting properties slightly better than those of the matrix. The filaments are assumed to result from inhomogeneities in the twophase Pb Bi alloys under investigation. The picture emerging by mid1935 was that, provided they were pure and free from strain, elemental superconductors exhibited complete flux exclusion, a reversible transition at a welldefined critical field, and a final state independent of the magnetization history. Alloys, on the other hand, showed gradual flux penetration starting at a field below, and finishing at a field somewhat higher, than the critical field typical of a pure element. In decreasing fields the magnetization of alloys was hysteretic, and residual trapped flux was often retained when the applied field had returned to zero. The socalled hard elemental superconductors such as Ta and Nb showed behavior similar to that of alloys. The research at Kharkov continued with careful magnetization measurements on single and polycrystalline pure metals, and on single alloy crystals of Pb Bi, Pb In, Pb Tl, and Hg Cd. Shubnikov s final contribution to the critical current story was systematic magnetization measurements on a series of PbTl single crystals of differing compositions. 29
4 716 Low Temp. Phys. 27 (99 10), September October 2001 D. DewHughes These showed that the change from ideal to alloy behavior occurred at a particular concentration of the alloying addition. For lesser concentrations the alloy behaved as a pure metal. As the concentration was increased above this particular value, the field at which flux began to penetrate decreased, and the field at which resistance was restored increased, with increasing concentration of alloying element. A clear picture of the change from what is now recognized as typei superconductor to typeii superconductor was presented, although there was an absence of crossreferencing between the Ukrainian and Western European work. The theoretical explanation of the two types of superconductor was still missing, as was any understanding of what really determined the critical current density. No further progress had been made on these two problems when once again work on superconductivity was frustrated by global conflict. THEORETICAL ADVANCES With the cessation of hostilities, renewed interest was taken in superconductivity. Helium gas was now much more readily available, its production having been accelerated by the needs of the US Navy for balloons. The development of the Collins liquefier allowed many more physics laboratories to indulge in studies at liquidhelium temperatures. However, the most startling advances were made on the theoretical front. In 1950 Ginsburg and Landau, at the Institute for Physical Problems in Moscow, published their phenomenological theory. 30 They ascribed to the superconductor an order parameter,, with some characteristics of a quantummechanical wave function. is a function of temperature and magnetic vector potential. The Gibbs function is expanded in even powers of about the transition temperature, as in Landau s theory of phase transitions, and terms to describe the magnetic energy and kinetic energy and momentum of the electrons are included in their expression for the Gibbs function of a superconductor in an external field. At an external surface their theory reproduces the results of the London theory. They introduced a new parameter, characteristic of a particular superconductor, & 2 q 0 H c /. The problem that they set out to solve, following the earlier speculations of H. London, was that of the surface energy between superconducting and normal regions in the same metal. Their results showed quite clearly that, if were to have a value greater than 1/&, then superconductivity could persist up to fields in excess of the critical field, given by H ( /&)H c. Ignoring the prewar work on alloys, they stated that for no superconductor was 0.1, and therefore this result was of no interest! Pippard, with wartime experience of microwave techniques, was now at Cambridge, engaged in measurements of microwave surface resistance in metals and superconductors. The anomalous skin effect in impure metals had been explained by nonlocal effects. The behavior of an electron was not influenced by the point value of the electric and magnetic fields but by the value averaged over a volume of dimensions equal to the electron mean free path l. By analogy with the explanation for the anomalous skin effect in metals, Pippard suggested that a similar nonlocality was appropriate to superconductors. In the London theory, the current density at a point r is determined by the value of the magnetic vector potential A(r). In Pippard s nonlocal modification of the London theory 31 the current density at r is determined by A averaged over a volume of dimensions 0. An electron traveling from a normal to a superconducting region cannot change its wave function abruptly; the change must take place over some finite distance. This distance is called the range of coherence, 0. Pippard estimated that, for pure or clean metals, 0 1 m. The Pippard theory introduces modifications to the penetration depth. For a clean superconductor, clean in this case meaning that the normal electron mean free path l 0, the penetration depth is given by )/2 0 L 2 1/3, 12 where L is the value of the penetration depth in the London theory. For alloy, or dirty superconductors, in which l 0, the theory gives a new, much greater, value for the penetration depth, L 0 /l 1/2, and also a much reduced value for the coherence length, d 0 l 1/ The Ginsburg Landau can be shown to be approximately equal to /, and for a dirty superconductor with l very small, i.e., high electrical resistivity in the normal state, can be quite large, e.g., 25 for niobiumbased alloys and compounds, and 100 for mixed oxide hightemperature superconductors. The next theoretical development was the formulation of the Bardeen Cooper Schrieffer BCS microscopic theory for superconductivity. 32 This theory, for which the authors received the 1972 Nobel Prize for Physics, is now the accepted theory for conventional superconductors. In superconductors below the transition temperature, electrons close to the Fermi surface condense into pairs Cooper pairs. These pairs are the charge carriers in superconductivity, and their charge q is equal to twice the charge on a single electron. The value of the flux quantum 0 h/2e Wb. The pairs form under an attractive interaction mediated by lattice phonons. An energy gap appears in the excitation spectrum for electrons at the Fermi level. Electron pairs, lattice phonons, and energy gaps in superconductivity had been postulated previously, but Bardeen, Cooper, and Schrieffer were the first to put all of these together in one theoretical framework. The energy gap is related to the critical temperature: 2 3.5kT c. 15 This represents the energy required to break up the Cooper pairs. It is possible to derive from this another estimate of the maximum current density, the depairing current. The depairing current density is that at which the kinetic energy of the superconducting carriers exceeds the binding energy of the Cooper pairs. It is then energetically favorable for the constituent electrons in a pair to separate and cease to be superconducting. The change in energy during scattering is maximized when the momentum change is maximized. This occurs when a carrier is scattered from one point on the
5 Low Temp. Phys. 27 (99 10), September October 2001 D. DewHughes 717 Fermi surface to a diametrically opposite one, in total reversal of direction. The carrier velocity is given by the sum of the drift and Fermi velocities; v d v f becomes v d v f. The resulting change in kinetic energy is E n 1 2 m v d v f m v d v f 2 2mv d v f. 16 The breaking of a pair followed by scattering causes a change in energy E s 2 2mv d v f. 17 For spontaneous depairing to occur, E s must be negative, i.e., the drift velocity must be greater than /mv f. The depairing current density J d, which is just the drift velocity times the carrier density n and the carrier charge q, must therefore be greater than J d nq /mv f. When appropriate substitutions are made this expression for J d can be shown to reduce to H c /, the previously quoted expression for the absolute maximum current density. Values of the depairing current density lie in the range A/m 2. Abrikosov, working in the same institute as Landau, made the fourth theoretical breakthrough in He produced a mathematical solution of the Ginsburg Landau equations for the case when 1/&. His solution showed that in a rising externally applied magnetic field, flux is excluded until a lower critical field, H c1, is exceeded. Above H c1 flux penetrates in the form of flux vortices, or flux lines, each carrying a quantum of flux 0, directed parallel to the field. The structure of these flux vortices is a normal core, of radius, containing the flux that is supported by supercurrents circulating over a radius. As the applied field is increased, more flux penetrates until the density of the flux lines is such that the normal cores begin to overlap. This occurs at the upper critical field, H c2 & H c0 0 / The regime between the lower and upper critical fields is known as the mixed state. The mutual repulsion between the flux vortices, in the absence of any other forces acting upon them, results in the formation of a triangular flux line lattice FLL. The parameter of this lattice is a ( 0 /B) 1/2, where B is the local value of the magnetic induction in the superconductor. Despite being published in translation, Abrikosov s paper took some time to be fully appreciated in the West. In 1960 Gor kov derived the constants in the Ginsburg Landau theory from the BCS theory. 34 This trilogy of Russian theoretical work is collectively referred to as the GLAG Ginsburg Landau Abrikosov Gor kov theory. Superconductors with values of 1/&, which exhibit the mixed state, are known as typeii superconductors. For any superconductor, as the normal state mean free path of the electrons, l, is reduced, gets smaller, gets larger, and increases. Alloying, by reducing l, raises. This explains Shubnikov s observation that the change from typei to typeii behavior, or the onset of the Shubnikov phase, occurs at a particular alloy concentration. 29 APPLIED SUPERCONDUCTIVITY The experimentalists had not been idle during this period. New superconductors, showing a steady increase in critical temperature, had been discovered: the brittle compounds NbN 15 K in 1941, V 3 Si(17 K) in 1951, Nb 3 Sn(18 K) in 1954, and the ductile alloys Nb Zr 11 K in 1953 and Nb Ti 10 K in All of these were typeii superconductors, with upper critical inductions well in excess of previously known materials. B c2 was about 12 T for Nb Ti and 25 T for Nb 3 Sn. The pioneers in this work were the groups at Westinghouse and Bell Telephone Laboratories. 2 Whereas the critical temperature and critical inductions were intrinsic properties of the superconductor, the critical current density was found to be strongly dependent upon the metallurgical state of the material. In twophase alloys J c was influenced by the size and dispersion of the second phase particles. 35 In the niobiumbased ductile BCC alloys, it was found 36 that cold deformation significantly enhanced J c. The problem of fabricating wire from the brittle intermetallic Nb 3 Sn was solved by filling niobium tubes with a mixture of Nb and Sn powders in the appropriate proportions, drawing to a fine wire, and reacting to form the compound. 37 This material had a current density of 10 9 A/m 2 in an induction of 8.8 T. Similar wire was wound into a solenoid which generated an induction of 2.85 T. 38 If the reaction to form the compound took place at the surface of the Nb and Sn particles, the compound could have formed as a threedimensional network, just as envisaged by Mendelssohn for his sponge. Could the twophase microstructure in the lead alloys, or the dislocations introduced by deformation of the ductile transition metal alloys, 39 constitute the elements of Mendelssohn s sponge? Or was there an alternative scenario? If the flux vortices in the mixed state were able to interact in some way with the microstructure, this interaction could impede both the ingress of flux in a rising field and the egress of flux in a falling field. This would lead to the magnetic hysteresis observed in the materials. Flux gradients resulting from nonuniform distributions of vortices can be equated with currents. A current flowing in a superconductor in the mixed state will exert a Lorentz force on the flux vortices, F L(V) J B per unit volume of superconductor, or F L(l) J 0 per unit length of vortex, where 0 is a vector of strength 0 directed along the vortex. The force acts in a direction normal to both flux and current. Unless otherwise prevented, the vortices will move in the direction of this force, and in so doing induce an electric field E v B, where v is the velocity of the vortices. The superconductor now shows an induced resistance, the value of which approaches that of the normal state, n, as the magnetic induction rises to B c2, the upper critical induction. 40 The critical current is that current at which a detectable voltage is produced across the superconductor, and is therefore that current which just causes the vortices to move. If there is no hindrance to the motion of the vortices, then above B c1 the critical current is zero and the magnetization is reversible. The moving vortices do experience a viscous drag, originating from dissipation in the normal cores. This force F v v, where the coefficient of viscosity 0 B/ n Ref. 40. If the vortices interact with microstructural features in the body of the superconductor, such as impurities, crystal defects, and secondphase precipitates, they can be prevented from moving and become pinned. The pinning force F p is a function of the microstruc
SUPERCONDUCTIVITY. PH 318 Introduction to superconductors 1
SUPERCONDUCTIVITY property of complete disappearance of electrical resistance in solids when they are cooled below a characteristic temperature. This temperature is called transition temperature or critical
More informationElectrical Conductivity
Advanced Materials Science  Lab Intermediate Physics University of Ulm Solid State Physics Department Electrical Conductivity Translated by MichaelStefan Rill January 20, 2003 CONTENTS 1 Contents 1 Introduction
More informationChapter Outline Dislocations and Strengthening Mechanisms
Chapter Outline Dislocations and Strengthening Mechanisms What is happening in material during plastic deformation? Dislocations and Plastic Deformation Motion of dislocations in response to stress Slip
More informationIntroduction to superconductivity
Introduction to superconductivity Textbook: Introduction to superconductivity by A.C.RoseInnes & E. H. Rhoderick 2 nd Ed. References: Introduction to superconductivity by M. Tinkham 2 nd Ed. superconductivity
More informationStructural Integrity Analysis
Structural Integrity Analysis 1. STRESS CONCENTRATION Igor Kokcharov 1.1 STRESSES AND CONCENTRATORS 1.1.1 Stress An applied external force F causes inner forces in the carrying structure. Inner forces
More informationSolid shape molding is not desired in injection molding due to following reasons.
PLASTICS PART DESIGN and MOULDABILITY Injection molding is popular manufacturing method because of its highspeed production capability. Performance of plastics part is limited by its properties which
More informationFundamentals of grain boundaries and grain boundary migration
1. Fundamentals of grain boundaries and grain boundary migration 1.1. Introduction The properties of crystalline metallic materials are determined by their deviation from a perfect crystal lattice, which
More informationXI / PHYSICS FLUIDS IN MOTION 11/PA
Viscosity It is the property of a liquid due to which it flows in the form of layers and each layer opposes the motion of its adjacent layer. Cause of viscosity Consider two neighboring liquid layers A
More informationphys4.17 Page 1  under normal conditions (pressure, temperature) graphite is the stable phase of crystalline carbon
Covalent Crystals  covalent bonding by shared electrons in common orbitals (as in molecules)  covalent bonds lead to the strongest bound crystals, e.g. diamond in the tetrahedral structure determined
More informationChapter Outline Dislocations and Strengthening Mechanisms
Chapter Outline Dislocations and Strengthening Mechanisms What is happening in material during plastic deformation? Dislocations and Plastic Deformation Motion of dislocations in response to stress Slip
More informationEðlisfræði 2, vor 2007
[ Assignment View ] [ Print ] Eðlisfræði 2, vor 2007 30. Inductance Assignment is due at 2:00am on Wednesday, March 14, 2007 Credit for problems submitted late will decrease to 0% after the deadline has
More informationEðlisfræði 2, vor 2007
[ Assignment View ] [ Pri Eðlisfræði 2, vor 2007 28. Sources of Magnetic Field Assignment is due at 2:00am on Wednesday, March 7, 2007 Credit for problems submitted late will decrease to 0% after the deadline
More information1. Fluids Mechanics and Fluid Properties. 1.1 Objectives of this section. 1.2 Fluids
1. Fluids Mechanics and Fluid Properties What is fluid mechanics? As its name suggests it is the branch of applied mechanics concerned with the statics and dynamics of fluids  both liquids and gases.
More informationTensile Testing. Objectives
Laboratory 1 Tensile Testing Objectives Students are required to understand the principle of a uniaxial tensile testing and gain their practices on operating the tensile testing machine. Students are able
More informationModule #17. Work/Strain Hardening. READING LIST DIETER: Ch. 4, pp. 138143; Ch. 6 in Dieter
Module #17 Work/Strain Hardening READING LIST DIETER: Ch. 4, pp. 138143; Ch. 6 in Dieter D. KuhlmannWilsdorf, Trans. AIME, v. 224 (1962) pp. 10471061 Work Hardening RECALL: During plastic deformation,
More informationPhysics 9e/Cutnell. correlated to the. College Board AP Physics 1 Course Objectives
Physics 9e/Cutnell correlated to the College Board AP Physics 1 Course Objectives Big Idea 1: Objects and systems have properties such as mass and charge. Systems may have internal structure. Enduring
More informationSteady Heat Conduction
Steady Heat Conduction In thermodynamics, we considered the amount of heat transfer as a system undergoes a process from one equilibrium state to another. hermodynamics gives no indication of how long
More informationProperties of Solids
Properties of Solids Condensed Matter Physics Condensed matter physics: The study of the electronic properties of solids. Crystal structure: The atoms are arranged in extremely regular, periodic patterns.
More informationIronCarbon Phase Diagram (a review) see Callister Chapter 9
IronCarbon Phase Diagram (a review) see Callister Chapter 9 University of Tennessee, Dept. of Materials Science and Engineering 1 The Iron Iron Carbide (Fe Fe 3 C) Phase Diagram In their simplest form,
More informationChapter 2. Derivation of the Equations of Open Channel Flow. 2.1 General Considerations
Chapter 2. Derivation of the Equations of Open Channel Flow 2.1 General Considerations Of interest is water flowing in a channel with a free surface, which is usually referred to as open channel flow.
More informationMSE 528  PRECIPITATION HARDENING IN 7075 ALUMINUM ALLOY
MSE 528  PRECIPITATION HARDENING IN 7075 ALUMINUM ALLOY Objective To study the time and temperature variations in the hardness and electrical conductivity of AlZnMgCu high strength alloy on isothermal
More informationCrystal Structure of High Temperature Superconductors. Marie Nelson East Orange Campus High School NJIT Professor: Trevor Tyson
Crystal Structure of High Temperature Superconductors Marie Nelson East Orange Campus High School NJIT Professor: Trevor Tyson Introduction History of Superconductors Superconductors are material which
More informationEnergy Transport. Focus on heat transfer. Heat Transfer Mechanisms: Conduction Radiation Convection (mass movement of fluids)
Energy Transport Focus on heat transfer Heat Transfer Mechanisms: Conduction Radiation Convection (mass movement of fluids) Conduction Conduction heat transfer occurs only when there is physical contact
More informationResistivity. V A = R = L ρ (1)
Resistivity Electric resistance R of a conductor depends on its size and shape as well as on the conducting material. The size and shapedependence was discovered by Georg Simon Ohm and is often treated
More informationLecture 19: Eutectoid Transformation in Steels: a typical case of Cellular
Lecture 19: Eutectoid Transformation in Steels: a typical case of Cellular Precipitation Today s topics Understanding of Cellular transformation (or precipitation): when applied to phase transformation
More informationElectromagnetism Laws and Equations
Electromagnetism Laws and Equations Andrew McHutchon Michaelmas 203 Contents Electrostatics. Electric E and Dfields............................................. Electrostatic Force............................................2
More informationDefects Introduction. Bonding + Structure + Defects. Properties
Defects Introduction Bonding + Structure + Defects Properties The processing determines the defects Composition Bonding type Structure of Crystalline Processing factors Defects Microstructure Types of
More informationEdmund Li. Where is defined as the mutual inductance between and and has the SI units of Henries (H).
INDUCTANCE MUTUAL INDUCTANCE If we consider two neighbouring closed loops and with bounding surfaces respectively then a current through will create a magnetic field which will link with as the flux passes
More informationNUMERICAL ANALYSIS OF THE EFFECTS OF WIND ON BUILDING STRUCTURES
Vol. XX 2012 No. 4 28 34 J. ŠIMIČEK O. HUBOVÁ NUMERICAL ANALYSIS OF THE EFFECTS OF WIND ON BUILDING STRUCTURES Jozef ŠIMIČEK email: jozef.simicek@stuba.sk Research field: Statics and Dynamics Fluids mechanics
More informationChapter Outline: Phase Transformations in Metals
Chapter Outline: Phase Transformations in Metals Heat Treatment (time and temperature) Microstructure Mechanical Properties Kinetics of phase transformations Multiphase Transformations Phase transformations
More informationBending, Forming and Flexing Printed Circuits
Bending, Forming and Flexing Printed Circuits John Coonrod Rogers Corporation Introduction: In the printed circuit board industry there are generally two main types of circuit boards; there are rigid printed
More informationPhysics 1653 Exam 3  Review Questions
Physics 1653 Exam 3  Review Questions 3.0 Two uncharged conducting spheres, A and B, are suspended from insulating threads so that they touch each other. While a negatively charged rod is held near, but
More informationIndiana's Academic Standards 2010 ICP Indiana's Academic Standards 2016 ICP. map) that describe the relationship acceleration, velocity and distance.
.1.1 Measure the motion of objects to understand.1.1 Develop graphical, the relationships among distance, velocity and mathematical, and pictorial acceleration. Develop deeper understanding through representations
More informationk u (t) = k b + k s t
Chapter 2 Stripe domains in thin films 2.1 Films with perpendicular anisotropy In the first part of this chapter, we discuss the magnetization of films with perpendicular uniaxial anisotropy. The easy
More informationLecture 8: Extrinsic semiconductors  mobility
Lecture 8: Extrinsic semiconductors  mobility Contents Carrier mobility. Lattice scattering......................... 2.2 Impurity scattering........................ 3.3 Conductivity in extrinsic semiconductors............
More informationAn equivalent circuit of a loop antenna.
3.2.1. Circuit Modeling: Loop Impedance A loop antenna can be represented by a lumped circuit when its dimension is small with respect to a wavelength. In this representation, the circuit parameters (generally
More informationFor Water to Move a driving force is needed
RECALL FIRST CLASS: Q K Head Difference Area Distance between Heads Q 0.01 cm 0.19 m 6cm 0.75cm 1 liter 86400sec 1.17 liter ~ 1 liter sec 0.63 m 1000cm 3 day day day constant head 0.4 m 0.1 m FINE SAND
More informationBasics of Superconducting Magnets
Basics of Superconducting Magnets The most basic of superconducting magnets is a simple solenoid in which a wire form of superconducting material is wound around a coil form. Various configurations of
More informationPPT No. 26. Uniformly Magnetized Sphere in the External Magnetic Field. Electromagnets
PPT No. 26 Uniformly Magnetized Sphere in the External Magnetic Field Electromagnets Uniformly magnetized sphere in external magnetic field The Topic Uniformly magnetized sphere in external magnetic field,
More informationChapter 4. Magnetic Materials and Circuits
Chapter 4 Magnetic Materials and Circuits Objectives List six characteristics of magnetic field. Understand the righthand rule for current and magnetic fluxes. Define magnetic flux, flux density, magnetomotive
More informationEXPERIMENTAL STUDY OF STRUCTURAL ZONE MODEL FOR COMPOSITE THIN FILMS IN MAGNETIC RECORDING MEDIA APPLICATION
EXPERIMENTAL STUDY OF STRUCTURAL ZONE MODEL FOR COMPOSITE THIN FILMS IN MAGNETIC RECORDING MEDIA APPLICATION Hua Yuan and David E. Laughlin Department of Materials Science and Engineering, Carnegie Mellon
More informationThe Kinetic Theory of Gases Sections Covered in the Text: Chapter 18
The Kinetic Theory of Gases Sections Covered in the Text: Chapter 18 In Note 15 we reviewed macroscopic properties of matter, in particular, temperature and pressure. Here we see how the temperature and
More informationPlate waves in phononic crystals slabs
Acoustics 8 Paris Plate waves in phononic crystals slabs J.J. Chen and B. Bonello CNRS and Paris VI University, INSP  14 rue de Lourmel, 7515 Paris, France chen99nju@gmail.com 41 Acoustics 8 Paris We
More informationDIRECT CURRENT GENERATORS
DIRECT CURRENT GENERATORS Revision 12:50 14 Nov 05 INTRODUCTION A generator is a machine that converts mechanical energy into electrical energy by using the principle of magnetic induction. This principle
More informationCLASSICAL CONCEPT REVIEW 8
CLASSICAL CONCEPT REVIEW 8 Kinetic Theory Information concerning the initial motions of each of the atoms of macroscopic systems is not accessible, nor do we have the computational capability even with
More information1. The diagram below represents magnetic lines of force within a region of space.
1. The diagram below represents magnetic lines of force within a region of space. 4. In which diagram below is the magnetic flux density at point P greatest? (1) (3) (2) (4) The magnetic field is strongest
More informationLecture 24  Surface tension, viscous flow, thermodynamics
Lecture 24  Surface tension, viscous flow, thermodynamics Surface tension, surface energy The atoms at the surface of a solid or liquid are not happy. Their bonding is less ideal than the bonding of atoms
More informationRef. Ch. 11 in Superalloys II Ch. 8 in Khanna Ch. 14 in Tien & Caulfield
MTE 585 Oxidation of Materials Part 1 Ref. Ch. 11 in Superalloys II Ch. 8 in Khanna Ch. 14 in Tien & Caulfield Introduction To illustrate the case of high temperature oxidation, we will use Nibase superalloys.
More informationChapter 14 Magnets and
Chapter 14 Magnets and Electromagnetism How do magnets work? What is the Earth s magnetic field? Is the magnetic force similar to the electrostatic force? Magnets and the Magnetic Force! We are generally
More information particle with kinetic energy E strikes a barrier with height U 0 > E and width L.  classically the particle cannot overcome the barrier
Tunnel Effect:  particle with kinetic energy E strikes a barrier with height U 0 > E and width L  classically the particle cannot overcome the barrier  quantum mechanically the particle can penetrated
More informationFatigue Testing. Objectives
Laboratory 8 Fatigue Testing Objectives Students are required to understand principle of fatigue testing as well as practice how to operate the fatigue testing machine in a reverse loading manner. Students
More informationDimensional Analysis
Dimensional Analysis An Important Example from Fluid Mechanics: Viscous Shear Forces V d t / / / / / / / / / / / / / / / / / / / / / / / / / / / / / / / / / Ƭ = F/A = μ V/d More generally, the viscous
More informationSolving Simultaneous Equations and Matrices
Solving Simultaneous Equations and Matrices The following represents a systematic investigation for the steps used to solve two simultaneous linear equations in two unknowns. The motivation for considering
More informationBasic Concepts of Thermodynamics
Basic Concepts of Thermodynamics Every science has its own unique vocabulary associated with it. recise definition of basic concepts forms a sound foundation for development of a science and prevents possible
More informationBoltzmann Distribution Law
Boltzmann Distribution Law The motion of molecules is extremely chaotic Any individual molecule is colliding with others at an enormous rate Typically at a rate of a billion times per second We introduce
More informationAP Physics 1 and 2 Lab Investigations
AP Physics 1 and 2 Lab Investigations Student Guide to Data Analysis New York, NY. College Board, Advanced Placement, Advanced Placement Program, AP, AP Central, and the acorn logo are registered trademarks
More informationVIII.4. Field Effect Transistors
Field Effect Transistors (FETs) utilize a conductive channel whose resistance is controlled by an applied potential. 1. Junction Field Effect Transistor (JFET) In JFETs a conducting channel is formed of
More informationQuestion 6.5: A steel bar 100 mm (4.0 in.) long and having a square cross section 20 mm
14:440:407 Ch6 Question 6.3: A specimen of aluminum having a rectangular cross section 10 mm 12.7 mm (0.4 in. 0.5 in.) is pulled in tension with 35,500 N (8000 lb f ) force, producing only elastic deformation.
More informationObjectives 200 CHAPTER 4 RESISTANCE
Objectives Explain the differences among conductors, insulators, and semiconductors. Define electrical resistance. Solve problems using resistance, voltage, and current. Describe a material that obeys
More information* Biot Savart s Law Statement, Proof Applications of Biot Savart s Law * Magnetic Field Intensity H * Divergence of B * Curl of B. PPT No.
* Biot Savart s Law Statement, Proof Applications of Biot Savart s Law * Magnetic Field Intensity H * Divergence of B * Curl of B PPT No. 17 Biot Savart s Law A straight infinitely long wire is carrying
More informationChapter Outline. Diffusion  how do atoms move through solids?
Chapter Outline iffusion  how do atoms move through solids? iffusion mechanisms Vacancy diffusion Interstitial diffusion Impurities The mathematics of diffusion Steadystate diffusion (Fick s first law)
More informationCh. 4: Imperfections in Solids Part 1. Dr. Feras Fraige
Ch. 4: Imperfections in Solids Part 1 Dr. Feras Fraige Outline Defects in Solids 0D, Point defects vacancies Interstitials impurities, weight and atomic composition 1D, Dislocations edge screw 2D, Grain
More informationCopyright 2011 Casa Software Ltd. www.casaxps.com. Centre of Mass
Centre of Mass A central theme in mathematical modelling is that of reducing complex problems to simpler, and hopefully, equivalent problems for which mathematical analysis is possible. The concept of
More informationContents. Goldstone Bosons in 3HeA Soft Modes Dynamics and Lie Algebra of Group G:
... Vlll Contents 3. Textures and Supercurrents in Superfluid Phases of 3He 3.1. Textures, Gradient Energy and Rigidity 3.2. Why Superfuids are Superfluid 3.3. Superfluidity and Response to a Transverse
More informationObjectives. Capacitors 262 CHAPTER 5 ENERGY
Objectives Describe a capacitor. Explain how a capacitor stores energy. Define capacitance. Calculate the electrical energy stored in a capacitor. Describe an inductor. Explain how an inductor stores energy.
More informationA Theoretical Model for Mutual Interaction between Coaxial Cylindrical Coils Lukas Heinzle
A Theoretical Model for Mutual Interaction between Coaxial Cylindrical Coils Lukas Heinzle Page 1 of 15 Abstract: The wireless power transfer link between two coils is determined by the properties of the
More informationemission of light from atoms discrete line spectra  energy levels, FranckHertz experiment
Introduction Until the early 20 th century physicists used to explain the phenomena in the physical world around them using theories such a mechanics, electromagnetism, thermodynamics and statistical physics
More informationLecture 6 Scanning Tunneling Microscopy (STM) General components of STM; Tunneling current; Feedback system; Tip  the probe.
Lecture 6 Scanning Tunneling Microscopy (STM) General components of STM; Tunneling current; Feedback system; Tip  the probe. Brief Overview of STM Inventors of STM The Nobel Prize in Physics 1986 Nobel
More informationPHYS 222 Spring 2012 Final Exam. Closed books, notes, etc. No electronic device except a calculator.
PHYS 222 Spring 2012 Final Exam Closed books, notes, etc. No electronic device except a calculator. NAME: (all questions with equal weight) 1. If the distance between two point charges is tripled, the
More informationDifferential Relations for Fluid Flow. Acceleration field of a fluid. The differential equation of mass conservation
Differential Relations for Fluid Flow In this approach, we apply our four basic conservation laws to an infinitesimally small control volume. The differential approach provides point by point details of
More informationMagnetism. d. gives the direction of the force on a charge moving in a magnetic field. b. results in negative charges moving. clockwise.
Magnetism 1. An electron which moves with a speed of 3.0 10 4 m/s parallel to a uniform magnetic field of 0.40 T experiences a force of what magnitude? (e = 1.6 10 19 C) a. 4.8 10 14 N c. 2.2 10 24 N b.
More informationLecture 3 Fluid Dynamics and Balance Equa6ons for Reac6ng Flows
Lecture 3 Fluid Dynamics and Balance Equa6ons for Reac6ng Flows 3. 1 Basics: equations of continuum mechanics  balance equations for mass and momentum  balance equations for the energy and the chemical
More informationQuestion Bank. 1. Electromagnetism 2. Magnetic Effects of an Electric Current 3. Electromagnetic Induction
1. Electromagnetism 2. Magnetic Effects of an Electric Current 3. Electromagnetic Induction 1. Diagram below shows a freely suspended magnetic needle. A copper wire is held parallel to the axis of magnetic
More information6 J  vector electric current density (A/m2 )
Determination of Antenna Radiation Fields Using Potential Functions Sources of Antenna Radiation Fields 6 J  vector electric current density (A/m2 ) M  vector magnetic current density (V/m 2 ) Some problems
More informationE/M Experiment: Electrons in a Magnetic Field.
E/M Experiment: Electrons in a Magnetic Field. PRELAB You will be doing this experiment before we cover the relevant material in class. But there are only two fundamental concepts that you need to understand.
More informationAS COMPETITION PAPER 2008
AS COMPETITION PAPER 28 Name School Town & County Total Mark/5 Time Allowed: One hour Attempt as many questions as you can. Write your answers on this question paper. Marks allocated for each question
More informationThe ASG s MRI 0.5T cryogenic free magnet
In spite of its recent discovery, MgB 2 has not only been routinely manufactured into long conductors, but useful examples of practical applications have been already realized. Some of them, using Columbus
More informationModule 1 : Conduction. Lecture 5 : 1D conduction example problems. 2D conduction
Module 1 : Conduction Lecture 5 : 1D conduction example problems. 2D conduction Objectives In this class: An example of optimization for insulation thickness is solved. The 1D conduction is considered
More informationExperimental Question 1: Levitation of Conductors in an Oscillating Magnetic Field SOLUTION ( )
a. Using Faraday s law: Experimental Question 1: Levitation of Conductors in an Oscillating Magnetic Field SOLUTION The overall sign will not be graded. For the current, we use the extensive hints in the
More informationNatural Convection. Buoyancy force
Natural Convection In natural convection, the fluid motion occurs by natural means such as buoyancy. Since the fluid velocity associated with natural convection is relatively low, the heat transfer coefficient
More informationLinear DC Motors. 15.1 Magnetic Flux. 15.1.1 Permanent Bar Magnets
Linear DC Motors The purpose of this supplement is to present the basic material needed to understand the operation of simple DC motors. This is intended to be used as the reference material for the linear
More informationThe Viscosity of Fluids
Experiment #11 The Viscosity of Fluids References: 1. Your first year physics textbook. 2. D. Tabor, Gases, Liquids and Solids: and Other States of Matter (Cambridge Press, 1991). 3. J.R. Van Wazer et
More informationFluids and Solids: Fundamentals
Fluids and Solids: Fundamentals We normally recognize three states of matter: solid; liquid and gas. However, liquid and gas are both fluids: in contrast to solids they lack the ability to resist deformation.
More informationINSTITUTE FOR APPLIED PHYSICS Physical Practice for Learners of Engineering sciences Hamburg University, Jungiusstraße 11
INSTITUTE FOR APPIED PHYSICS Physical Practice for earners of Engineering sciences Hamburg University, Jungiusstraße 11 Hall effect 1 Goal Characteristic data of a test semiconductor (Germanium) should
More informationSize effects. Lecture 6 OUTLINE
Size effects 1 MTX9100 Nanomaterials Lecture 6 OUTLINE Why does size influence the material s properties? How does size influence the material s performance? Why are properties of nanoscale objects
More informationGear Trains. Introduction:
Gear Trains Introduction: Sometimes, two or more gears are made to mesh with each other to transmit power from one shaft to another. Such a combination is called gear train or train of toothed wheels.
More informationDC GENERATOR THEORY. LIST the three conditions necessary to induce a voltage into a conductor.
DC Generators DC generators are widely used to produce a DC voltage. The amount of voltage produced depends on a variety of factors. EO 1.5 LIST the three conditions necessary to induce a voltage into
More informationSURFACE TENSION. Definition
SURFACE TENSION Definition In the fall a fisherman s boat is often surrounded by fallen leaves that are lying on the water. The boat floats, because it is partially immersed in the water and the resulting
More informationStudents Manual for the Exam
Students Manual for the Exam General Engineering and Mechanical Engineering Discipline  March 2014  COPYRIGHT NOTICE COPYRIGHTS 2013 NATIONAL CENTER FOR ASSESSMENT IN HIGHER EDUCATION (QIYAS) UNLESS
More informationCHARGE TO MASS RATIO OF THE ELECTRON
CHARGE TO MASS RATIO OF THE ELECTRON In solving many physics problems, it is necessary to use the value of one or more physical constants. Examples are the velocity of light, c, and mass of the electron,
More informationPROPERTIES OF MATERIALS
1 PROPERTIES OF MATERIALS 1.1 PROPERTIES OF MATERIALS Different materials possess different properties in varying degree and therefore behave in different ways under given conditions. These properties
More informationLecture 18 Strain Hardening And Recrystallization
138 Lecture 18 Strain Hardening And Recrystallization Strain Hardening We have previously seen that the flow stress (the stress necessary to produce a certain plastic strain rate) increases with increasing
More information develop a theory that describes the wave properties of particles correctly
Quantum Mechanics Bohr's model: BUT: In 192526: by 1930s:  one of the first ones to use idea of matter waves to solve a problem  gives good explanation of spectrum of single electron atoms, like hydrogen
More informationAjit Kumar Patra (Autor) Crystal structure, anisotropy and spin reorientation transition of highly coercive, epitaxial PrCo films
Ajit Kumar Patra (Autor) Crystal structure, anisotropy and spin reorientation transition of highly coercive, epitaxial PrCo films https://cuvillier.de/de/shop/publications/1306 Copyright: Cuvillier Verlag,
More informationLecture 5 Hemodynamics. Description of fluid flow. The equation of continuity
1 Lecture 5 Hemodynamics Description of fluid flow Hydrodynamics is the part of physics, which studies the motion of fluids. It is based on the laws of mechanics. Hemodynamics studies the motion of blood
More informationPhysics 41, Winter 1998 Lab 1  The Current Balance. Theory
Physics 41, Winter 1998 Lab 1  The Current Balance Theory Consider a point at a perpendicular distance d from a long straight wire carrying a current I as shown in figure 1. If the wire is very long compared
More informationPhysics 126 Practice Exam #3 Professor Siegel
Physics 126 Practice Exam #3 Professor Siegel Name: Lab Day: 1. Which one of the following statements concerning the magnetic force on a charged particle in a magnetic field is true? A) The magnetic force
More informationAPPLICATION NOTE Innovative shunt design techniques optimise power measurement accuracy
APPLICATION NOTE  012 Innovative shunt design techniques optimise power measurement accuracy Introduction Rapid developments in power conversion technologies combined with a need for better product efficiency
More informationPrelab Exercises: Hooke's Law and the Behavior of Springs
59 Prelab Exercises: Hooke's Law and the Behavior of Springs Study the description of the experiment that follows and answer the following questions.. (3 marks) Explain why a mass suspended vertically
More informationChapter Outline. Mechanical Properties of Metals How do metals respond to external loads?
Mechanical Properties of Metals How do metals respond to external loads? Stress and Strain Tension Compression Shear Torsion Elastic deformation Plastic Deformation Yield Strength Tensile Strength Ductility
More information